JCP O-90 Printable Plastic Film (Synthetic Paper) February 1, 2008 

Miscellaneous Paper FSC 9310 

 

Use Information: This paragraph is informational only and is not exclusively definitive of the end use. 

For multicolor face and back offset printing of manuals, maps, tags, outdoor billboards, etc., requiring a high degree of tear 
resistance including resistance to action of water, mild aqueous solutions, grease, oils, extreme climatic temperatures, frequent 
handling, discoloration and durability. Printed matter may include text, line illustrations, and halftones up to 175-line screen. 

 

Stock: Shall be a non-cellulose substrate. 

Note: Recovered material, in any percentage, is 
encouraged, provided that the requirements of this 
Standard are met. 

 

Such as -- 

PPG Teslin R SP (www.teslin.com) 

Arjobex Polyart R (www.polyart.com) 

YUPO R (www.yupo.com) 

AET SynCarta tm SLC (www.syncarta.com) 

HOP-SYN R II DURA-LITE (www.hopindustries.com) 

 

 

Caliper: Nominal (mils) 

4 

5.5 

7 

8.5 



 

 

Folding endurance: Average each direction not 
less than (MIT double folds) ................. 

 
4,000 

 

Aged film1: Average each direction not less than 
50% of the unaged film or (MIT double folds)  

 

 

4,000 



 

Opacity: Average not less than 
(percent)  

 

90 

 

92 

 

94 

 

96 



 

Surface: The film shall not flake, powder, crack, blister, 
or otherwise deteriorate under print or other handling 
conditions, shall not discolor, become brittle, or be subject 
to attack by mold, mildew, or fungus under normal 
conditions, and shall be uniform, free from mottle, and 
from any particles that will pick, lift, fluff, or pile on use 
under normal conditions. 

 

Aged film1: The L* component of the color shall not 
decrease more than 3 percentage points. 

 

General appearance: Film shall conform to the standard 
sample(s) established by the Government. 

Brightness: Shall not less than target 88% or as specified. 

Color: The paper in the order (or publication) shall be 
uniform and the color variation shall not exceed 
DE(CIELAB) = 1.0. 

Finish and formation: Shall be uniform. 

Cleanliness: The film shall be clean. 

 

Testing: Shall be conducted in accordance with methods in part 2, Government Paper Specification Standards. The 
acceptance criteria Part 4 does not apply. 

 

 

 

 

 

 

 

 

 

 

 

 

 

 

 

 

 

 

 

 

 

 

___________ 

1 Age material for 48 hours in an Atlas fadeometer or equivalent with a carbon arc